Review Article  Open Access
Multiple Exciton Generation in Nanostructures for Advanced Photovoltaic Cells
Abstract
This paper reviews both experimental and theoretical work on nanostructures showing high quantum yields due to the phenomenon of multiple exciton generation. It outlines the aims and barriers to progress in identifying further such nanostructures and also includes important developments concerning solar devices where nanostructures act as the lightabsorbing component. It reports on both semiconductor and carbon structures, both monocomposite (of various dimensionalities) and heterogeneous. Finally, it looks at future directions that can be taken to push solar cell efficiency above the classic limit set by Shockley and Queisser in 1961.
1. Introduction
Current solar energy conversion inefficiency is considered by many to be the greatest barrier to sustainably meet modern day energy needs. Since the early 20th century, there has been an increasing interest in solar voltaics, with early models of pn junction solar cells manufactured since the 1950s (Figure 1). In 1961, Shockley and Queisser discovered a fundamental limit to the efficiency of a traditional pn solar cell of 30% [1]. At the end of the 20th century, secondgeneration solar cells were manufactured which use multiple layers of the semiconducting material. These devices absorb a greater range of frequencies and do surpass this limit, pushing the theoretical limit to a 68% efficiency. However, the manufacture of such multijunction solar cells is too expensive for largescale commercial use [2]. Theory and experiments show that there is potential to overcome the Shockley–Queisser limit using quantum effects for a new cheap thirdgeneration solar cell [3, 4] (Figure 2). In fact, it is known that impact ionisation in bulk semiconductor materials allows for hot excitons to relax to the valence band, in turn exciting another exciton (Figure 3). However, in bulk, this does not occur at the typical frequencies of solar photons. Therefore, intensive research is being done with the aim of increasing the quantum yield (QY) of photovoltaic cells by enhancing biexciton creation in nanostructures, which allow for a significant response to a wider frequency spectrum. Such structures include nanosheets or “platelets,” nanorods, nanowires, and, notably, quantum dots (QDs). In nanostructures, electronhole pair multiplication, whereby more than one (typically two) electronhole pairs are generated by impact with a single incoming photon, is referred to as multiple exciton generation (MEG), to differentiate it from bulk impact ionisation. Let us mention that alternative terminologies, such as “carrier multiplication” (CM) or “multiple exciton collection” (MEC), are also in use in the literature. It is also worth knowing that zerodimensional structures (quantum dots) may also be referred to as “nanocrystals.”
(a)
(b)
This review paper is organised as follows: in Section 2, the notion of multiple exciton generation is cursorily recalled, along with some basic related terminologies; Section 3 covers MEG in zerodimensional (quantum dots) structures, with an emphasis on Pb and Sibased dots; Section 4 moves onto onedimensional structures, in particular, to nanorods, nanotubes, and nanoribbons; Section 5 is devoted to twodimensional structures, such as generic nanosheets and graphene sheets; Section 6 completes our survey focusing on hybrid type II heterostructures, which have drawn interest in this context; finally, in Section 7, we include a summary and a few conclusive remarks.
2. Multiple Exciton Generation
The creation of additional carriers from hot excitons has been observed in bulk semiconductors such as PbS, PbSe, and Si [7] and was not included in the seminal analysis by Shockley and Queisser. Theoretical work by De Vos et al. has, however, shown that a QY higher than unity is beneficial for increasing solar device efficiency [8–11]. In a pn junction solar cell, it has been shown that efficient impact ionisation occurs when the incident photon energy is in excess of five times the energy required to excite an exciton to the valence band, leading to quantum efficiencies above unity [12, 13]. Typically, this is highenergy ultraviolet light outside the solar spectrum. Hence, a key aim in order to exploit this effect is to reduce the threshold energy for it to take place so that quantum yields (i.e., the number of excitons per incoming photon) greater than unity can be reached with solar photons. Before 2002, MEG was often referred to as “downshifting” or “downconversion” of hot excitons, and devices were theorized, which would facilitate this process [14, 15]. In 2002, however, Nozik was the first to propose that MEG could be enhanced by using nanostructures [16]. Research published soon after by Shaller and Klimov showed evidence for lowthreshold MEG in PbSe QDs [17]. Since then, MEG has been observed repeatedly in a variety of QDs such as PbSe [2], PbS [18], and eSi [19], while some semiconductor QDs such as eInAs have, as of yet, shown no signs of MEG [1, 20, 21]. Notably, MEG has also been demonstrated in C structures, such as nanotubes, nanoribbons, and graphene [22].
It is worth noticing that such studies are typically carried out in a colloidal environment, using either photoluminescence, transient absorption, or, more recently, pumpprobe spectroscopy. All of these methods are labour intensive and difficult, and, indeed, the lack of quick and easy MEG tests is arguably one of the major barriers in the field [23]. As a consequence, it is only recently that nanostructures have been put into actual devices. The study of such devices is arguably a new field in itself, involving practical and technical considerations that elude the main scope of this review. Although we shall mention several of the most important advances concerning devices, the reader is referred to [24] for a more detailed and exhaustive account.
The early reported QYs of experiments (2005–2010) varied widely up to extremes of 300% [19, 25–27]. It was later discovered that some suspiciously optimistic results were due to photocharging, whereby electrons delocalise from the parent QDs. This gives a deceptive MEGlike signature in the spectroscopic data. Subsequently, it was found that this effect could be nullified simply by stirring the sample solution [28]. Another hurdle in the assessment of QYs for specific structures is clearly the large number of variables involved and relevant to these effects, such as the size, composition, shape, and method of observation. It is uncommon for studies to be done on likeforlike samples so that corroborative results are rare [29]. The complicated interplay between the phonon cooling rate and the nanostructure dimensions is also an important reason for the wide variety in reported QY values [30]. In fact, there is still no general, unified theoretical framework for describing MEG. Nevertheless, all of the studies in the area agree on two key factors: the enhancement of the Coulombic coupling between exciton and biexciton states and the suppression of excitons’ radiative relaxation pathways (predominantly phonon emission) are critical for increasing QY [5, 6, 31, 32]. Such conditions can be achieved by reducing the size of the basic structures, as quantum confinement favours both of them.
As far as the general theory of MEG is concerned, it should be noted that the intriguing possibility of mechanisms hinging on coherent superpositions of multiple excitonic states has been put forward, but it does not agree with all experiments [25, 33]. More recently “window of opportunity” models have been used [34, 35], which allow for more predictive power than previous modelling. They rely on splitting relaxation times into discrete amounts and are often complemented with computer simulations. The main aim of these studies is identifying conditions whereby the threshold photon energy for multiple excitations, , and the electronhole pair energy (the energy required for a further exciton to be created) are minimised. In the ideal case scenario, they would approach the limit set by the conservation of energy, when and , with being the bandgap energy. This produces a staircase function when plotting pump energy against QY, which is often taken as an optimal reference.
It should be mentioned that when discussing in situ structures, the observed QY is sometimes also termed “quantum efficiency.” When dealing with devices, however, one is typically interested only in their quantum efficiency. This is further qualified as either “external” or “internal” quantum efficiency. The former is the ratio of generated electrons to incident photons, whilst the latter is the ratio of electrons to absorbed photons, which takes into account reflection and transmission, and is always lower. Furthermore, let us remark that, in understanding the relationship between in situ structures and devices, the exciton lifetime τ plays a key role, as a larger τ allows for excitons to be “collected,” thus increasing the device’s quantum efficiency.
3. Quantum Dots
Due to their comparative topological simplicity and ease of fabrication, QDs are the best understood class of nanostructures. It is thus not surprising that efforts have been made to design effective ways to assemble devices from QDs and for turning excitons into carriers [36].
In order to be competitive candidates for solar voltaic devices, QDs must have within the infrared region, high QY, and be stable in the cell environment. For these reasons, PbS, PbSe, PbTe, Si, and TiO_{2} QDs have received the most attention (Figure 4). Computational methods are used in order to identify further possible options [5, 37]. Typically, such methods adopt densityfunctional theory, which provides a satisfactory compromise between accuracy and scale. In Si_{29}H_{36}, the MEG dynamics in QDs was probed using densityfunctional theory [38], placing the threshold for efficient MEG at about which, for Si_{29}H_{36}, lies within the visible spectrum. Such computational techniques are bound to furnish additional insight as methods and machines improve. On the other hand, computational methods are typically not designed explicitly to resolve the excited states occupied by biexcitons, which poses challenges and limitations to this approach.
As pointed out above, it is important that photovoltaic structures exhibit quantum confinement. In this regard, theory suggests that, for this to be the case, the radius of the QD should be less than the bulk exciton Bohr radius, calculated as , with ε and μ being, respectively, the dielectric constant and the reduced mass of the electron and hole. Typical values for such Bohr radii are , , and [40]. QDs of these sizes can now by synthesised easily.
3.1. PbX Quantum Dots
Leadbased QDs have been studied intensively, as here is in the low infrared spectrum, fabrication is easily scalable, reproducible, and low cost, and, most importantly, the Bohr exciton radius tends to be large. After initial studies in 2009, it was doubted that PbSe QDs, which, it should be mentioned, feature the added complication of being unstable in air, would exhibit MEG at all [17, 41]. However, in 2010, Beard et al. [12] showed sufficient evidence for MEG, and now, PbSe QDs are possibly the most studied structures in this arena. In 2014, an improvement in PbSe synthesis was introduced that allowed the QDs to survive for up to thirty days in air, showing an increase of orders of magnitude over previous lifetimes [42]. This was made possible by a novel synthetic method whereby PbSe QDs are made directly from CdSe QDs by displacing the Cd with Pb, creating a protective Cl and Cd ion surface on the subsequent PbSe QD film. (In order to check that the other characteristics of the QD films were the same as standard ones, direct comparisons were carried out, showing that the MEG dynamics are unchanged.)
In a 2016 study, the QY of PbSe QDs of three different sizes was determined (Table 1) [30], for radii of 1.8 ± 0.2 nm, 1.9 ± 0.3 nm, and 2.2 ± 0.3 nm, respectively, all much smaller than the PbSe Bohr radius and thus in the strong quantum confinement region. The peaks in transition absorption observed in the experiment may be associated with specific, previously known orbital energies [43]. In particular, the socalled transitions to the “Brillouin Zone” (unique to PbSe), a set of electronic transitions where MEG is expected to be particularly strong due to an enhanced phonon bottleneck, were investigated by probing the biexciton dynamics through transient absorption. The measures of the QY of each QD at three different pump energies thus highlighted the central role played by electron excitation to the levels in increasing efficiency, in agreement with the related theory.

PbX QDs share similar crystal structure, and so, systematic, comparative investigations may be launched where the second element is changed, in order to isolate the impact of different variables on the overall yields [44]. A 2011 study made the comparison between PbSe and PbS to determine why QY for PbSe seemed much higher [45]. These two QDs are studied particularly as PbS QDs are stable in air and have the same structure as PbSe QDs which, as already mentioned, are relatively unstable in air. By looking at excitedstate lifetimes, it was established that the excitonbiexciton Coulomb coupling was very similar in both QDs. After observing a dependency of QY on the QD size for PbS but not for PbSe, it was also possible to infer that other relaxation channels, specifically the phonon relaxation rate, must be the dominant factor at play in determining the different QYs. This result was instrumental in leading to the first mediumscale collection of QY data on a variety of leadbased QDs of different sizes [44] (Figure 5). In this paper, the accompanying theory is refined with the introduction of the parameters η, an MEG efficiency value independent of the pump rate, and , a factor which describes the competition between the rate of MEG and the rate of nonuseful cooling . In PbSe, MEG occurs at about , which is described by a η value between 0.4 and 0.5 (Figure 6). The following empirical equation relates with the photon energies involved:where s is a factor which describes how MEG changes with and the excess pump photon energy . Here, s is found to be around 2.2 for leadbased QDs. The study by Midgett et al. [28] and Mihaylov et al. [38] in agreement with previous relevant literature also reports on properties for a variety of PbS_{x}Se_{1−x} alloy QDs, with varying composition and radius, allowing one to draw conclusions about the size dependence of η for the different compositions of QDs (Figure 6). It is suggested that higher MEG might be achievable in nonspherical crystal structures, although more data need to be collected to explore such configurations.
3.2. Si Quantum Dots
Silicon is abundant in nature. It makes up over 90% of solar voltaic devices currently in use and plays a huge role in electronics and technology. It poses no environmental issues, and Si membranes are optically transparent to nonbandgap energy photons, such that it would be possible to create Si multilayer cells of different sizes in order to span a wider absorption spectrum and achieve greater efficiency [46]. It also has within the infrared, making it potentially an ideal material for thirdgeneration solar cells.
QY above unity with silicon QDs was first reported in 2007 by Beard et al. [19] who tested QDs of two different diameters: one in the strong confinement region (below the Bohr exciton radius for Si of 4.9 nm) and the other in the weakintermediate confinement region (about double the Bohr exciton radius). MEG was thus observed in a colloidal environment for both of these QDs at a pump energy of 0.86 eV. The reconstructed value for the electronhole energy was (close to the energy conservation limit of ), with a reported QY of 2.3 ± 0.2 at . Other relaxation pathways other than phonon emission were also taken into account in this study, such as charge transfer and radiative recombination [3].
In 2016, Bergren et al. used pumpprobe spectroscopy to study a range of differently sized Si QDs [47]. As will be discussed below, in recent years, emphasis has been on trying to extend biexciton lifetimes, which is the angle taken by Bergren et al. in this work. Thus, they found that, as one should expect, biexciton lifetimes increase as the diameter is reduced, and postulate that the increase in the quantum confinement is reducing the coupling to the phonon relaxation channels. This is consistent with evidence for other QDs.
Study of Si QD films is also intensive due to easy access to highgrade samples. In [48], a novel way to induce MEG in an array of Si QDs was described, showing that if the QDs are in close proximity, hot excitons can excite excitons in neighbouring QDs rather than in their parent QDs. Specifically, this experiment used Si QDs of around 1.8 nm embedded in an SiO_{2} matrix. MEG obtained through such a thermal exciton propagation enjoys a reduced chance of Auger recombination, and exciton lifetime prolonged by up to six orders of magnitude. A recent paper by Kryjevski and Kilin [49] adopts densityfunctional theory to evaluate the effect of changing the internal structure of the QDs in amorphous QDs, as opposed to crystalline ones: such computer simulations predict a considerable change in dynamics in the twodimensional density limit present in films. They suggest that, in this case, amorphous QDs may show a marked improvement in QY, along with better carrier mobility.
Recently, research has increasingly focused on novel structures rather than on mere manipulation of the QD size. The production and characterisation of all multilayer Si cells with different bandgaps due to different levels of P dopant, rather than due to different sizes, have been first explored [46]. High levels of MEG in GeX QDs and higher QYs than in bulk GeX were subsequently observed in these structures [50], with external quantum efficiency exceeding 120% for PbTe QDs [51]. It is perhaps worth noting that such studies, which focus on external QYs, are key to showing that the in situ study feature behaviours can be replicated for realworld usage.
4. OneDimensional Structures
Over the last few years, onedimensional structures have started to draw attention as candidates for photovoltaic devices alternative to quantum dots. Whilst clearly more challenging to synthesise than zerodimensional dots, higherdimensional structures entail a breaking of the spherical symmetry that lifts some of the energy level degeneracies and thus allows for additional excitations. Besides, theoretical models suggested that, despite the increased volume of onedimensional structures such as nanorods, they would still lie in the quantum confinement region, as the effect of quantum confinement depends not merely on the total volume of a structure but rather on its effective crosssectional area [52, 53]. In terms of MEG, nanowires have only been considered in preliminary computational studies [38, 49]. On the other hand, cell architectures based on nanorods and nanotubes have received some attention [54].
4.1. Nanorods
Pbbased nanorods were the first nonspherical structures to be studied for MEG, which was made possible by synthetic methods developed in 2010 [55, 56]. Initial reports showed the first evidence of MEG [57, 58]. In particular, in a paper by Cunningham et al. [58], values of and close to the ideal values of and were reported. The key issue in these studies is clearly to achieve a general understanding of the effect of length and aspect ratio on QYs. The PbSe nanorods’ QY dependence on the aspect ratio (defined as ) was investigated soon afterwards [39, 59], indicating that higher efficiency may be due to increased exciton Coulombic couplings at certain ρ, as suggested in [52]. After testing samples with different ρ and , it was found that the QY has a nonlinear, nonmonotonic dependence with ρ, and η, displaying an almost threefold increase at certain ρ values (Figure 7); in particular, the efficiency peaks at ρ = 67 give a twofold increase in the QY over PbSe QDs. The “enhancement factor” (defined as for the same composition) varies significantly across the literature. In late 2015, Davis et al. measured an external quantum efficiency exceeding unity for PbSe nanorods [60]. More specifically, external QYs of 109 ± 3%, 113 ± 3%, and 122 ± 3% were measured for devices containing nanorods of , , and . This is a promising result, which gives confidence that the same structures could be used in future devices. In the same study, the internal QY is shown to be in very good agreement with preexisting experimental and theoretical literature [59, 61].
(a)
(b)
4.2. Carbon Nanotubes and Nanoribbons
Theoretical work from 2004 suggested that strong Coulombic interactions between carriers would be present in singlewalled carbon nanotubes (SWCNTs) [63, 64]. This and other characteristics such as interesting photo and electric properties, as well as strong photon absorption, imply that such structures have the potential for MEG. Despite being considered a 1D material, the dynamics that governs MEG in SWCNTs is different to nanorods or nanowires. This is because excitons are confined to the surface of the SWCNTs rather than at their centre, which implies a quasi2D behaviour.
An initial 2008 study tested a SWCNT sample with mixed chiralities [65] showing a QY of 130% for . A paper published two years later performed the same experiment with SWCNTs of specific chiralities [66]. The latter, by Wang et al., achieved the same QY at for [7, 8] SWCNTs. However, both these results show values of outside the solar spectrum. Biexciton creation was further reported in 2013 [67], although no QY is quoted there. A basic hurdle toward the exploitation of SWCNTs in photovoltaic cells is represented by the difficulty of synthesing samples of a single chirality, which require labourintensive retroprocesses. For more information about the uses of SWCNTs in the solar voltaic system outside of enhancing MEG, see [68, 69].
Recently, MEG has been investigated in graphene nanoribbons (GNRs) using transient absorption [70]. GNRs have the advantage of having synthesis methods of atomic precision [71]. Furthermore, MEG turns out to be enhanced in these structures compared to SWCNTs, as they can be made extremely narrow with a significantly smaller surface area per unit length. The study of GNRs may still be considered to be in its infancy. However, initial theoretical reports indicate potential for extraordinary photoelectric properties [72–74].
5. Nanosheets
Synthetic methods for semiconductor nanosheets are still imprecise and difficult, and as such, they are the greatest barrier to their study [75]. In 2014, Aerts et al. [76] used a method of synthesis described in [77] to make ultrathin PbS nanosheets and test them via transient absorption (Figure 8). Sheets of three thickness, 4.0 ± 0.1, 5.9 ± 0.1, and 7.0 ± 0.1 nm, gave values for the maximum transient absorption bleaching (measure of the proportion of absorbed photons, where T is temperature), which could be inserted into the equationto determine the QY, . The transient bleach cross section was determined from lowenergy pumping with a known incident number of photons per unit area. The data analysis shows the notable result that is not affected by the nanosheet’s thickness or . Most remarkably, it also shows that, for the thinnest nanosheet of 4 nm, one has . This is extremely close to the optimal value of and would suggest that all excess energy has gone into exciting multiple carriers. Note that this is significantly larger than the reported values for PbX QDs, which is around η = 0.3–0.5 [41, 44, 59]. Unfortunately, these nanosheets have the disadvantage of high , although the ability to exhibit nearperfect efficiency once the threshold frequencies are reached is extremely interesting per se.
(a)
(b)
(c)
5.1. Graphene
A more readily available 2D structure with wellestablished synthesis is graphene, whose promise for useful optoelectric properties, such as high carrier densities and charge mobility, is well known [78]. Between 2010 and 2012, theoretical work by Winzer et al. showed that graphene has the potential for MEG [79, 80]. Only a year later, Tielrooij et al. [81] carried out a study on MEG biexciton creation in graphene through methods similar to those that would then be used in [76] on PbSe nanosheets. Such a study identifies two dominant processes: carriercarrier scattering, leading to MEG, and phononassisted cooling, as well as a branching ratio between the two, which is shown to be highly favourable for MEG. This study employed doped graphene and suggests a dependence of the results on the doping levels, which would open the additional possibility to alter the threshold energies for MEG by changing the amount of dopant as with Si. Soon after, in 2014, MEG was detected in lowdoped graphene too [82].
It should be mentioned that graphene has been studied in a wide variety of roles inside devices, not only as the lightabsorbing component. To find out more about its role in enhancing photoinduced voltage in dyesensitised solar cells and QD cells, see the review paper [83].
6. Type II Heterostructures
New QD structures that aim to separate the hole and electron wave functions have emerged recently. The wave function separation suppresses Auger recombination and thus increases the exciton lifetime [34]. These “type II” heterostructures are created by using multiple different compositions in the same structure (Figure 9).
A prominent example of a heterostructure is represented by coreshell QDs, such as those studied in the work of Cirloganu et al. in [84], on the basis of a phenomenological model for MEG proposed by Stewart et al. [35], which suggests that slowing down hot carrier relaxation might be even more important than previously thought. In general, this work has spurred an interest in coolingrate engineering for nanostructures, and in turn, much research into how the separation between electron and hole wave functions may be increased.
Cirloganu et al. propose that the electron wave functions are spread over the whole structure, while the hole wave functions are localised around the core, creating the desired spatial separation, and proceed to study QDs with a PbSe core and a CdSe shell of varying sizes; such dots can be characterised by an aspect ratio ρ, defined as the ratio of shell thickness to the overall radius. Thus, consistently higher MEG rates than reported for PbSe QDs were observed for coreshell QDs. A critical aspect ratio, which would provide the energyconservation limit of η = 1, is predicted to lie in the interval ρ_{c }= 0.45–0.7. Further related analysis on the effect of coreshell aspect ratio, as well as of the degree of alloying between the core and the shell and its spectrographic implications, can be found in the review [85].
In the same year, Eshet et al. looked at heterostructured nanorods of CdSe and CdS [86] created by a seededgrowth approach [87]. They analysed both seeded and coreshell structures, obtaining results which comply with the standard behaviour above : for the seeded structures, the efficiency η increases with the seed size, while for the core/shell structures, η increases as the core diameter decreases. However, when probing the samples in the nonMEG regime , it was found that, unexpectedly, η actually decreases with decreasing core size, which is converse to theoretical prediction as well as monocomposite QD behaviour. A 2016 paper by Eshet et al. furthered the inquiry into how could be lowered from previous values of around by analysing the dynamics of nanorod heterostructures whose composition changes from one to the other end of the rod. The theory suggests that, in this class of heterostructures, the internal electric field generated from photon pumping would aid MEG. When pumping around the energy conservation limit of , MEG efficiencies of 10%–20% were observed.
No semiconductor heterostructures were investigated in 2Dconfined systems. However, there has been research into the socalled “Van der Waals” graphene heterostructures [88] (Figure 10). These consist of layers of graphene separated by nanosheets of other materials, such as MoS_{2} or WSe_{2}. MEG studies on this kind of “material stacks” proved inconclusive [89], and further research is needed to shed light as to their potential.
7. Summary and Outlook
The technology required to create new generations of cheap and efficient solar cells is still a way off its ultimate goal. Despite this, since 2002, there have been significant breakthroughs in the study of nanostructures to overcome the Shockley–Queisser limit. Through generating multiple pairs of excitons per incident photon, efficiencies have been measured strongly, indicating that this goal should be achievable. As this compact review strived to show, experimental progress has led to a better understanding of the dynamics which governs excitons experiencing zero, one, and twodimensional quantum confinement. Work by computational and theoretical groups has led to research which allows for better prediction in future candidates for MEG and better prediction of the effect various factors such as aspect ratio or size might have.
Quantum dots in a colloidal environment have now moved onto being studied in device environments. To some extent, monocomposite QDs are being put to one side in favour of studies into heterostructures. The most stateoftheart and applicable results have come from the creation of actual devices and measurement of high external quantum efficiencies [42, 51, 60]. Whilst they have yet to show voltages exceeding the Shockley–Queisser limit, such devices have given external QYs showing that MEG does work when turning excitons into carriers. To these aims, the potential of carbon structures is still not well understood in the one and twodimensional regimes. However, research has conclusively shown that higherdimensional architectures do reach extremely high efficiencies at threshold frequencies outside the solar spectrum [82, 90]. Attempts to reduce the threshold energy by using ribbons, multilayers of graphene, and other systems are underway.
Future investigation into the possibility of creating nanorod and nanosheet devices seems to be in order, as well as into the effect of the nanostructure environment on the MEG efficiency. In particular, a better understanding of the latter seems to be a key to really appreciate the impact these combined advances might have toward potentially revolutionary results. It should also be noted that MEG itself is unlikely to be the only pathway toward thirdgeneration solar cells. It is one of the many phenomena being explored that could come together in order to create such devices. It seems fair to predict that when this research is combined with other work into the effect of electric fields on solar voltaic performance, or tandem cells, the application of nanostructures to light harvesting might achieve enhanced efficiencies in both proofofprinciple experiments and operational devices in the short or medium term.
Conflicts of Interest
The authors declare that there are no conflicts of interest regarding the publication of this paper.
Acknowledgments
The authors acknowledge financial support from EPSRC through grant EP/K026267/1.
References
 W. Shockley and H. J. Queisser, “Detailed balance limit of efficiency of pn junction solar cells,” Journal of Applied Physics, vol. 32, no. 3, pp. 510–519, 1961. View at: Publisher Site  Google Scholar
 F. C. Krebs, J. Fyenbo, and M. Jorgensen, “Product integration of compact rolltoroll processed polymer solar cell modules: methods and manufacture using flexographic printing, slotdie coating and rotary screen printing,” Journal of Materials Chemistry, vol. 20, no. 41, pp. 8994–9001, 2010. View at: Publisher Site  Google Scholar
 M. O. Scully, “Quantum photocell: using quantum coherence to reduce radiative recombination and increase efficiency,” Physical Review Letters, vol. 104, no. 20, pp. 1–4, 2010. View at: Publisher Site  Google Scholar
 P. Krogstrup, H. I. Jørgensen, M. Heiss et al., “Singlenanowire solar cells beyond the Shockley–Queisser limit,” Nature Photonics, vol. 7, no. 4, pp. 306–310, 2013. View at: Publisher Site  Google Scholar
 H. M. Jaeger, K. I. M. Hyeondeuk, and O. V. Prezhdo, “Exciton multiplication from first principles,” Accounts of Chemical Research, vol. 46, no. 6, pp. 1280–1289, 2013. View at: Publisher Site  Google Scholar
 A. Shabaev, C. S. Hellberg, and A. L. Efros, “Efficiency of multiexciton generation in colloidal nanostructures,” Accounts of Chemical Research, vol. 46, no. 6, pp. 1242–1251, 2013. View at: Publisher Site  Google Scholar
 D. J. Robbins, “Aspects of the theory of impact ionization in semiconductors (I),” Physica Status Solidi (B), vol. 97, no. 1, pp. 9–50, 1980. View at: Publisher Site  Google Scholar
 V. Badescu, P. T. Landsberg, A. De Vos, and B. Desoete, “Statistical thermodynamic foundation for photovoltaic and photothermal conversion. IV. Solar cells with largerthanunity quantum efficiency revisited,” Journal of Applied Physics, vol. 89, no. 4, pp. 2482–2490, 2001. View at: Publisher Site  Google Scholar
 A. De Vos and B. Desoete, “On the ideal performance of solar cells with largerthanunity quantum efficiency,” Solar Energy Materials and Solar Cells, vol. 51, no. 34, pp. 413–424, 1998. View at: Publisher Site  Google Scholar
 A. De Vos, P. T. Landsberg, P. Baruch, and J. E. Parrott, “Entropy fluxes, endoreversibility, and solar energy conversion,” Journal of Applied Physics, vol. 74, no. 6, pp. 3631–3637, 1993. View at: Publisher Site  Google Scholar
 P. Baruch, A. De Vos, P. T. Landsberg, and J. E. Parrott, “On some thermodynamic aspects of photovoltaic solar energy conversion,” Solar Energy Materials and Solar Cells, vol. 36, no. 2, pp. 201–222, 1995. View at: Publisher Site  Google Scholar
 M. C. Beard, A. G. Midgett, M. C. Hanna, J. M. Luther, B. K. Hughes, and A. J. Nozik, “Comparing multiple exciton generation in quantum dots to impact ionization in bulk semiconductors: implications for enhancement of solar energy conversion,” Nano Letters, vol. 10, no. 8, pp. 3019–3027, 2010. View at: Publisher Site  Google Scholar
 S. Kolodinski, J. H. Werner, T. Wittchen, and H. J. Queisser, “Quantum efficiencies exceeding unity due to impact ionization in silicon solar cells,” Applied Physics Letters, vol. 63, no. 17, pp. 2405–2407, 1993. View at: Publisher Site  Google Scholar
 T. Trupke, M. A. Green, and P. Würfel, “Improving solar cell efficiencies by downconversion of highenergy photons,” Journal of Applied Physics, vol. 92, no. 3, pp. 1668–1674, 2002. View at: Publisher Site  Google Scholar
 V. Badescu, A. De Vos, A. M. Badescu, and A. Szymanska, “Improved model for solar cells with downconversion and downshifting of highenergy photons,” Journal of Physics D: Applied Physics, vol. 40, no. 2, pp. 341–352, 2007. View at: Publisher Site  Google Scholar
 A. J. Nozik, “Quantum dot solar cells,” Physica E: LowDimensional Systems and Nanostructures, vol. 14, no. 12, pp. 115–120, 2002. View at: Publisher Site  Google Scholar
 R. D. Schaller and V. I. Klimov, “High efficiency carrier multiplication in PbSe nanocrystals: implications for solar energy conversion,” Physical Review Letters, vol. 92, no. 18, p. 186601, 2004. View at: Publisher Site  Google Scholar
 R. D. Schaller, M. Sykora, J. M. Pietryga, and V. I. Klimov, “Seven excitons at a cost of one: redefining the limits for conversion efficiency of photons into charge carriers,” Nano Letters, vol. 6, no. 3, pp. 424–429, 2006. View at: Publisher Site  Google Scholar
 M. C. Beard, K. P. Knutsen, P. Yu et al., “Multiple exciton generation in colloidal silicon nanocrystals,” Nano Letters, vol. 7, no. 8, pp. 2506–2512, 2007. View at: Publisher Site  Google Scholar
 G. Nair and M. G. Bawendi, “Carrier multiplication yields of CdSe and CdTe nanocrystals by transient photoluminescence spectroscopy,” Physical Review B, vol. 76, no. 8, p. 81304, 2007. View at: Publisher Site  Google Scholar
 J. J. H. Pijpers, E. Hendry, M. T. W. Milder et al., “Carrier multiplication and its reduction by photodoping in colloidal InAs quantum dots,” Journal of Physical Chemistry C, vol. 111, no. 11, pp. 4146–4152, 2007. View at: Publisher Site  Google Scholar
 N. M. Gabor, Z. Zhong, K. Bosnick, J. Park, and P. L. McEuen, “Extremely efficient multiple electronhole pair generation in carbon nanotube photodiodes,” Science, vol. 325, no. 5946, pp. 1367–1371, 2009. View at: Publisher Site  Google Scholar
 J. Gao, A. F. Fidler, and V. I. Klimov, “Carrier multiplication detected through transient photocurrent in devicegrade films of lead selenide quantum dots,” Nature Communications, vol. 6, p. 8185, 2015. View at: Publisher Site  Google Scholar
 C. J. Stolle, T. B. Harvey, and B. A. Korgel, “Nanocrystal photovoltaics : a review of recent progress,” Current Opinion in Chemical Engineering, vol. 2, no. 2, pp. 160–167, 2013. View at: Publisher Site  Google Scholar
 R. Ellingson, M. Beard, J. Johnson et al., “Highly efficient multiple exciton generation in colloidal PbSe and PbS quantum dots,” Nano Letters, vol. 5, no. 5, pp. 865–871, 2005. View at: Publisher Site  Google Scholar
 M. C. Beard, “Multiple exciton generation in semiconductor quantum dots,” Journal of Physical Chemistry Letters, vol. 2, no. 11, pp. 1282–1288, 2011. View at: Publisher Site  Google Scholar
 J. A. McGuire, M. Sykora, J. Joo, J. M. Pietryga, and V. I. Klimov, “Apparent versus true carrier multiplication yields in semiconductor nanocrystals,” Nano Letters, vol. 10, no. 6, pp. 2049–2057, 2010. View at: Publisher Site  Google Scholar
 A. G. Midgett, H. W. Hillhouse, B. K. Hughes, A. J. Nozik, and M. C. Beard, “Flowing versus static conditions for measuring multiple exciton generation in PbSe quantum dots,” Journal of Physical Chemistry C, vol. 114, no. 41, pp. 17486–17500, 2010. View at: Publisher Site  Google Scholar
 Y. Kanai, Z. Wu, and J. C. Grossman, “Charge separation in nanoscale photovoltaic materials: recent insights from firstprinciples electronic structure theory,” Journal of Materials Chemistry, vol. 20, no. 6, pp. 1053–1061, 2010. View at: Publisher Site  Google Scholar
 M. Kumar, S. Vezzoli, Z. Wang et al., “Hot exciton cooling and multiple exciton generation in PbSe quantum dots,” Physical Chemistry Chemical Physics, vol. 18, no. 45, pp. 31107–31114, 2016. View at: Publisher Site  Google Scholar
 A. Piryatinski and K. A. Velizhanin, “An exciton scattering model for carrier multiplication in semiconductor nanocrystals: theory,” Journal of Chemical Physics, vol. 133, no. 8, p. 084508, 2010. View at: Publisher Site  Google Scholar
 A. Le Bris and J. F. Guillemoles, “Hot carrier solar cells: achievable efficiency accounting for heat losses in the absorber and through contacts,” Applied Physics Letters, vol. 97, no. 11, pp. 2010–2013, 2010. View at: Publisher Site  Google Scholar
 A. Shabaev, A. L. Efros, and A. J. Nozik, “Multiexciton generation by a single photon in nanocrystals,” Nano Letters, vol. 6, no. 12, pp. 2856–2863, 2006. View at: Publisher Site  Google Scholar
 A. Piryatinski, S. A. Ivanov, S. Tretiak, and V. I. Klimov, “Effect of quantum and dielectric confinement on the exciton–exciton interaction energy in type II core/shell semiconductor nanocrystals,” Nano Letters, vol. 7, no. 1, pp. 108–115, 2007. View at: Publisher Site  Google Scholar
 J. T. Stewart, L. A. Padilha, W. K. Bae, W. K. Koh, J. M. Pietryga, and V. I. Klimov, “Carrier multiplication in quantum dots within the framework of two competing energy relaxation mechanisms,” Journal of Physical Chemistry Letters, vol. 4, no. 12, pp. 2061–2068, 2013. View at: Publisher Site  Google Scholar
 X. Lan, S. Masala, and E. H. Sargent, “Chargeextraction strategies for colloidal quantum dot photovoltaics,” Nature Materials, vol. 13, no. 3, pp. 233–240, 2014. View at: Publisher Site  Google Scholar
 I. M. Georgescu, S. Ashhab, and F. Nori, “Quantum simulation,” Reviews of Modern Physics, vol. 86, no. 1, pp. 153–185, 2014. View at: Publisher Site  Google Scholar
 D. Mihaylov, A. Kryjevski, D. Kilin, S. Kilina, and D. Vogel, “Multiple Exciton Generation in Semiconductor Nanostructures: DFTbased Computation,” in Proceedings of APS March Meeting, Baltimore, Maryland, March 2016. View at: Google Scholar
 L. A. Padilha, J. T. Stewart, R. L. Sandberg et al., “Carrier multiplication in semiconductor nanocrystals: influence of size, shape, and composition,” Accounts of Chemical Research, vol. 46, no. 6, pp. 1261–1269, 2013. View at: Publisher Site  Google Scholar
 M. C. Beard, H. I. P. Alexander, J. M. Luther, E. H. Sargent, and A. J. Nozik, “Quantum confined semiconductors for enhancing solar photoconversion through multiple exciton generation,” in Advanced Concepts in Photovoltaics, pp. 345–378, RSC Publishing, Cambridge, UK, 2014. View at: Publisher Site  Google Scholar
 J. J. H. Pijpers, R. Ulbricht, K. J. Tielrooij et al., “Assessment of carriermultiplication efficiency in bulk PbSe and PbS,” Nature Physics, vol. 5, no. 11, pp. 811–814, 2009. View at: Publisher Site  Google Scholar
 J. Zhang, J. Gao, C. P. Church et al., “PbSe quantum dot solar cells with more than 6% efficiency fabricated in ambient atmosphere,” Nano Letters, vol. 14, no. 10, pp. 6010–6015, 2014. View at: Publisher Site  Google Scholar
 R. Koole, G. Allan, C. Delerue, A. Meijerink, D. Vanmaekelbergh, and A. J. Houtepen, “Optical investigation of quantum confinement in PbSe nanocrystals at different points in the Brillouin zone,” Small, vol. 4, no. 1, pp. 127–133, 2008. View at: Publisher Site  Google Scholar
 A. G. Midgett, J. M. Luther, J. T. Stewart et al., “Size and composition dependent multiple exciton generation efficiency in PbS, PbSe, and PbS,” Nano Letters, vol. 13, no. 7, pp. 3078–3085, 2013. View at: Publisher Site  Google Scholar
 J. T. Stewart, L. A. Padilha, M. M. Qazilbash et al., “Comparison of carrier multiplication yields in PbS and PbSe nanocrystals: the role of competing energyloss processes,” Nano Letters, vol. 12, no. 2, pp. 622–628, 2012. View at: Publisher Site  Google Scholar
 X. J. Hao, E. C. Cho, G. Scardera et al., “Phosphorusdoped silicon quantum dots for allsilicon quantum dot tandem solar cells,” Solar Energy Materials and Solar Cells, vol. 93, no. 9, pp. 1524–1530, 2009. View at: Publisher Site  Google Scholar
 M. R. Bergren, P. K. B. Palomaki, N. R. Neale, T. E. Furtak, and M. C. Beard, “Sizedependent exciton formation dynamics in colloidal silicon quantum dots,” ACS Nano, vol. 10, no. 2, pp. 2316–2323, 2016. View at: Publisher Site  Google Scholar
 M. T. Trinh, R. Limpens, W. D. A. M. de Boer, J. M. Schins, L. D. A. Siebbeles, and T. Gregorkiewicz, “Direct generation of multiple excitons in adjacent silicon nanocrystals revealed by induced absorption,” Nature Photonics, vol. 6, no. 5, pp. 316–321, 2012. View at: Publisher Site  Google Scholar
 A. Kryjevski and D. Kilin, “Enhanced multiple exciton generation in amorphous silicon nanowires and films,” Molecular Physics, vol. 114, no. 34, pp. 365–379, 2015. View at: Publisher Site  Google Scholar
 S. Saeed, C. de Weerd, P. Stallinga et al., “Carrier multiplication in germanium nanocrystals,” Light: Science and Applications, vol. 4, no. 2, p. e251, 2015. View at: Publisher Site  Google Scholar
 M. L. Bohm, T. C. Jellicoe, M. Tabachnyk et al., “Lead telluride quantum dot solar cells displaying external quantum efficiencies exceeding 120%,” Nano Letters, vol. 15, no. 12, pp. 7987–7993, 2015. View at: Publisher Site  Google Scholar
 A. C. Bartnik, A. L. Efros, W. K. Koh, C. B. Murray, and F. W. Wise, “Electronic states and optical properties of PbSe nanorods and nanowires,” Physical Review BCondensed Matter and Materials Physics, vol. 82, no. 19, pp. 1–16, 2010. View at: Publisher Site  Google Scholar
 L. S. Li, J. Hu, W. Yang, and A. P. Alivisatos, “Band gap variation of size and shapecontrolled colloidal CdSe quantum rods,” Nano Letters, vol. 1, no. 7, pp. 349–351, 2001. View at: Publisher Site  Google Scholar
 E. C. Garnett, M. L. Brongersma, Y. Cui, and M. D. Mcgehee, “Nanowire solar cells,” Annual Reviews of Materials Research, vol. 41, pp. 269–295, 2011. View at: Publisher Site  Google Scholar
 W. K. Koh, A. C. Bartnik, F. W. Wise, and C. R. B. Murray, “Synthesis of monodisperse PbSe nanorods: a case for oriented attachment,” Journal of the American Chemical Society, vol. 132, no. 11, pp. 3909–3913, 2010. View at: Publisher Site  Google Scholar
 H. Wang, Y. Liu, M. Li et al., “Facile synthesis of ultrasmall PbSe nanorods for photovoltaic application,” Optoelectronics and Advanced Materials, Rapid Communications, vol. 4, no. 8, pp. 1166–1169, 2010. View at: Google Scholar
 R. L. Sandberg, L. A. Padilha, M. M. Qazilbash et al., “Multiexciton dynamics in infraredemitting colloidal nanostructures probed by a superconducting nanowire singlephoton detector,” ACS Nano, vol. 6, no. 11, pp. 9532–9540, 2012. View at: Publisher Site  Google Scholar
 P. D. Cunningham, J. E. Boercker, E. E. Foos et al., “Enhanced multiple exciton generation in quasionedimensional semiconductors,” Nano Letters, vol. 11, no. 8, pp. 3476–3481, 2011. View at: Publisher Site  Google Scholar
 L. A. Padilha, J. T. Stewart, R. L. Sandberg et al., “Aspect ratio dependence of auger recombination and carrier multiplication in PbSe nanorods,” Nano Letters, vol. 13, no. 3, pp. 1092–1099, 2013. View at: Publisher Site  Google Scholar
 N. J. L. K. Davis, M. L. Bo, M. Tabachnyk et al., “Multipleexciton generation in lead selenide nanorod solar cells with external quantum efficiencies exceeding 120%,” Nature Communications, vol. 6, no. 2, pp. 137–141, 2015. View at: Publisher Site  Google Scholar
 P. Cunningham, J. Boercker, E. Foos et al., “Correction to enhanced multiple exciton generation in quasionedimensional semiconductors,” Nano Letters, vol. 13, no. 6, p. 3003, 2013. View at: Publisher Site  Google Scholar
 J. A. McGuire, J. Joo, J. M. Pietryga, R. D. Schaller, and V. I. Klimov, “New aspects of carrier multiplication in semiconductor nanocrystals,” Accounts of Chemical Research, vol. 41, no. 12, pp. 1810–1819, 2008. View at: Publisher Site  Google Scholar
 C. Spataru, S. IsmailBeigi, L. Benedict, and S. Louie, “Excitonic effects and optical spectra of singlewalled carbon nanotubes,” Physical Review Letters, vol. 92, no. 7, p. 077402, 2004. View at: Publisher Site  Google Scholar
 V. Perebeinos, J. Tersoff, and P. Avouris, “Scaling of excitons in carbon nanotubes,” Physical Review Letters, vol. 92, no. 25, p. 257402–1, 2004. View at: Publisher Site  Google Scholar
 A. Ueda, K. Matsuda, T. Tayagaki, and Y. Kanemitsu, “Carrier multiplication in carbon nanotubes studied by femtosecond pumpprobe spectroscopy,” Applied Physics Letters, vol. 92, no. 23, p. 233105, 2008. View at: Publisher Site  Google Scholar
 S. Wang, M. Khafizov, X. Tu, M. Zheng, and T. D. Krauss, “Multiple exciton generation in singlewalled carbon nanotubes,” Nano Letters, vol. 10, no. 7, pp. 2381–2386, 2010. View at: Publisher Site  Google Scholar
 B. Yuma, S. Berciaud, J. Besbas et al., “Biexciton, single carrier, and trion generation dynamics in singlewalled carbon nanotubes,” Physical Review BCondensed Matter and Materials Physics, vol. 87, no. 20, pp. 1–7, 2013. View at: Publisher Site  Google Scholar
 D. D. Tune and J. G. Shapter, “The potential sunlight harvesting efficiency of carbon nanotube solar cells,” Energy and Environmental Science, vol. 6, no. 9, pp. 2572–2577, 2013. View at: Publisher Site  Google Scholar
 D. Jariwala, V. K. Sangwan, L. J. Lauhon, T. J. Marks, and M. C. Hersam, “Carbon nanomaterials for electronics, optoelectronics, photovoltaics, and sensing,” Chemical Society Reviews, vol. 42, no. 7, pp. 2824–2860, 2013. View at: Publisher Site  Google Scholar
 G. Soavi, S. Dal Conte, C. Manzoni et al., “Excitonexciton annihilation and biexciton stimulated emission in graphene nanoribbons,” Nature Communications, vol. 7, p. 11010, 2016. View at: Publisher Site  Google Scholar
 J. Cai, P. Ruffieux, R. Jaafar et al., “Atomically precise bottomup fabrication of graphene nanoribbons,” Nature, vol. 466, no. 7305, pp. 470–473, 2010. View at: Publisher Site  Google Scholar
 D. Prezzi, D. Varsano, A. Ruini, and E. Molinari, “Quantum dot states and optical excitations of edgemodulated graphene nanoribbons,” Physical Review BCondensed Matter and Materials Physics, vol. 84, no. 4, pp. 1–4, 2011. View at: Publisher Site  Google Scholar
 L. Yang, M. L. Cohen, and S. G. Louie, “Excitonic effects in the optical spectra of graphene nanoribbons,” Nano Letters, vol. 7, no. 10, pp. 3112–3115, 2007. View at: Publisher Site  Google Scholar
 D. Prezzi, D. Varsano, A. Ruini, A. Marini, and E. Molinari, “Optical properties of graphene nanoribbons: the role of manybody effects,” Physical Review B, vol. 77, no. 4, p. 41404, 2007. View at: Publisher Site  Google Scholar
 M. Nasilowski, B. Mahler, E. Lhuillier, S. Ithurria, and B. Dubertret, “Twodimensional colloidal nanocrystals,” Chemical Reviews, vol. 116, no. 18, pp. 10934–10982, 2016. View at: Publisher Site  Google Scholar
 M. Aerts, T. Bielewicz, C. Klinke et al., “Highly efficient carrier multiplication in PbS nanosheets,” Nature Communications, vol. 5, p. 3789, 2014. View at: Publisher Site  Google Scholar
 C. Schliehe, B. H. Juarez, M. Pelletier et al., “Ultrathin PbS sheets by twodimensional oriented attachment,” Science, vol. 329, no. 5991, pp. 550–553, 2010. View at: Publisher Site  Google Scholar
 F. Bonaccorso, Z. Sun, T. Hasan, and A. C. Ferrari, “Graphene photonics and optoelectronics,” Nature Photonics, vol. 4, no. 9, pp. 611–622, 2010. View at: Publisher Site  Google Scholar
 T. Winzer, A. Knorr, and E. Malic, “Carrier multiplication in graphene,” Nano Letters, vol. 10, no. 12, pp. 4839–4843, 2010. View at: Publisher Site  Google Scholar
 T. Winzer and E. Malić, “Impact of Auger processes on carrier dynamics in graphene,” Physical Review BCondensed Matter and Materials Physics, vol. 85, no. 24, pp. 1–5, 2012. View at: Publisher Site  Google Scholar
 K. J. Tielrooij, J. C. W. Song, S. A. Jensen et al., “Photoexcitation cascade and multiple hot carrier generation in graphene,” in 2013 Conference on Lasers and ElectroOptics Europe and International Quantum Electronics Conference, CLEO/EuropeIQEC, Munich, Germany, May 2013. View at: Publisher Site  Google Scholar
 T. Plötzing, T. Winzer, E. Malic, D. Neumaier, A. Knorr, and H. Kurz, “Experimental verification of carrier multiplication in graphene,” Nano Letters, vol. 14, no. 9, pp. 5371–5375, 2014. View at: Publisher Site  Google Scholar
 C. A. Ubani, M. A. Ibrahim, M. A. M. Teridi, K. Sopian, J. Ali, and K. T. Chaudhary, “Application of graphene in dye and quantum dots sensitized solar cell,” Solar Energy, vol. 137, pp. 531–550, 2016. View at: Publisher Site  Google Scholar
 C. M. Cirloganu, L. A. Padilha, Q. Lin et al., “Enhanced carrier multiplication in engineered quasitypeII quantum dots,” Nature Communications, vol. 5, p. 4148, 2014. View at: Publisher Site  Google Scholar
 V. I. Klimov, “Multicarrier interactions in semiconductor nanocrystals in relation to the phenomena of auger recombination and carrier multiplication,” Annual Review of Condensed Matter Physics, vol. 5, no. 1, pp. 285–316, 2014. View at: Publisher Site  Google Scholar
 H. Eshet, R. Baer, D. Neuhauser, and E. Rabani, “Theory of highly efficient multiexciton generation in typeII nanorods,” Nature Communications, vol. 7, p. 13178, 2016. View at: Publisher Site  Google Scholar
 L. Carbone, C. Nobile, M. De Giorgi et al., “Synthesis and micrometerscale assembly of colloidal CdSe/CdS nanorods prepared by a seeded growth approach,” Nano Letters, vol. 7, no. 10, pp. 2942–2950, 2007. View at: Publisher Site  Google Scholar
 A. K. Geim and I. V. Grigorieva, “Van der Waals heterostructures,” Nature, vol. 499, no. 7459, pp. 419–425, 2014. View at: Publisher Site  Google Scholar
 S. Wu, L. Wang, Y. Lai et al., “Multiple hotcarrier collection in photoexcited graphene Moiré superlattices,” Science Advances, vol. 2, no. 5, p. e1600002, 2016. View at: Publisher Site  Google Scholar
 J. McClain and J. Schrier, “Multiple exciton generation in graphene nanostructures,” Journal of Physical Chemistry C, vol. 114, no. 34, pp. 14332–14338, 2010. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2018 Nicholas Siemons and Alessio Serafini. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.